All Two-Dimensional, Flexible, Transparent, and Thinnest Thin Film Transistor Saptarshi Das,*,†,‡ Richard Gulotty,†,§ Anirudha V. Sumant,*,† and Andreas Roelofs† †
Center for Nanoscale Material, Argonne National Laboratory, Argonne, Illinois 60439, United States Birck Nanotechnology Center, Purdue University, West Lafayette, Indiana 47907, United States § Materials Science and Engineering Program, Bourns College of Engineering, University of California − Riverside, Riverside, California 92521 United States ‡
S Supporting Information *
ABSTRACT: In this article, we report only 10 atomic layer thick, high mobility, transparent thin ﬁlm transistors (TFTs) with ambipolar device characteristics fabricated on both a conventional silicon platform as well as on a ﬂexible substrate. Monolayer graphene was used as metal electrodes, 3−4 atomic layers of h-BN were used as the gate dielectric, and ﬁnally bilayers of WSe2 were used as the semiconducting channel material for the TFTs. The ﬁeld eﬀect carrier mobility was extracted to be 45 cm2/(V s), which exceeds the mobility values of state of the art amorphous silicon based TFTs by ∼100 times. The active device stack of WSe2−hBN− graphene was found to be more than 88% transparent over the entire visible spectrum and the device characteristics were unaltered for in-plane mechanical strain of up to 2%. The device demonstrated remarkable temperature stability over 77−400 K. Low contact resistance value of 1.4 kΩ-μm, subthreshold slope of 90 mv/decade, current ON−OFF ratio of 107, and presence of both electron and hole conduction were observed in our all two-dimensional (2D) TFTs, which are extremely desirable but rarely reported characteristics of most of the organic and inorganic TFTs. To the best of our knowledge, this is the ﬁrst report of all 2D transparent TFT fabricated on ﬂexible substrate along with the highest mobility and current ON−OFF ratio. KEYWORDS: 2D Crystal, graphene, thin ﬁlm transistor, ﬂexible electronics
One of the most promising applications of optimally stacked 2D materials is as thin ﬁlm transistors (TFT). The recent outburst of the display technology has made it even more appealing because the light emitting diodes (LEDs) and liquid crystal displays (LCDs) are driven by TFTs. TFTs are also used in RFID tags, ﬂexible electronic devices, and for sensing applications. Although, the thin ﬁlm transistor industry is reasonably mature, it is nowhere close to the ultimate potential due to limited material choices. Amorphous silicon (a-Si) is the most popular and widely used material for the TFTs.18,19 Numerous organic and inorganic materials had also been extensively explored.20−23 However, search for the better materials is still on. The most desirable features of TFTs are high carrier mobility, high ON−OFF current ratio, low contact resistance, presence of both electron and hole conduction, high optical transparency, temperature stability, and mechanical ﬂexibility.24 The 2D layered materials are a natural choice for the TFTs in order to meet these requirements. Moreover, their inherent electrostatic integrity allows them to operate at low
wo dimensional (2D) layered materials like graphene, hexagonal boron nitride (h-BN), and transition metal dichalcogenides (TMDs) are receiving signiﬁcant attention across all scientiﬁc disciplines due to their unique electrical, mechanical, thermal, and optical properties.1−12 High carrier velocity, exceptional mechanical stability, and near invisibility of graphene had already resulted in its commercialization as stretchable and transparent electrodes and interconnects.1−4 Graphene has also been substantially investigated as an alternative to silicon for beyond CMOS nanoelectronics. However, the absence of a sizable bandgap prevents the use of graphene in the logic circuits and has paved the way for the exploration of semiconducting TMDs like MoS2, WSe2, MoSe2, among others. Several high-performance ﬁeld eﬀect transistors (FETs) based on TMDs have been demonstrated in the recent literature.7−12 Various studies also indicate the potential of TMDs for optical, mechanical, chemical, and thermal applications.13−17 Finally, h-BN complements both, highly conductive graphene and semiconducting TMDs, not only by being a large bandgap insulator, but also, often as a substrate with better interface qualities.5,6 Integrating the unique properties of these diﬀerent 2D materials therefore provides numerous possibilities to shape the future of nanoelectronics. © 2014 American Chemical Society
Received: March 10, 2014 Revised: April 15, 2014 Published: April 22, 2014 2861
dx.doi.org/10.1021/nl5009037 | Nano Lett. 2014, 14, 2861−2866
Figure 1. (a) False color SEM image (b) 3D cartoon, and (c) cross sectional view of an all 2D TFT with graphene as metal electrode, h-BN as gate dielectric and WSe2 as the semiconducting channel material.
underlying WSe2 acts as just an additional dielectric layer. Figure 2c shows the position of the Fermi level inside graphene in response to the applied back gate bias screened by bilayer WSe2. We have used the Landauer formalism for current transport and taken into account the quantum capacitance contribution in order to solve the self-consistent Poisson equation to calculate ΨGRAPHENE. The details can be found elsewhere.25−27 Our numerical calculations backed by experimental observations suggest that the Fermi level in graphene can be moved by ∼300 meV on either side of the Dirac point over the applied gate bias range.28,29 This is an important ﬁnding in the context of graphene to WSe2 contact as will be discussed next. The presence of both the electron and the hole conduction in our WSe2 thin ﬁlm transistor (Figure 2a) strongly suggests that the Dirac point of graphene aligns close to the middle of the bandgap of WSe2. Because the bandgap of bilayer WSe2 is ∼1.3 eV, this would indicate the existence of large Schottky barrier heights at graphene to WSe2 contacts for both electron injection into the conduction band (ΦN0) and hole injection into the valence band (ΦP0) as shown in the associated band diagram in Figure 2d (brown box). When a negative gate bias is applied, the energy bands in WSe2 bend to facilitate hole injection into the valence band and at the same time the Fermi level in graphene also moves closer to the valence band, thereby reducing the eﬀective Schottky barrier height for hole injection to ΦP as shown in the purple box in Figure 2d. Similarly for positive gate bias, the energy bands in WSe2 bend to facilitate electron injection into the conduction band and at the same time the Fermi level in graphene also moves closer to the conduction band, thereby reducing the eﬀective Schottky barrier height for electron injection to ΦN as shown in the black box in Figure 2d. Using the technique proposed by Das11 and adjusting the eﬀective bandgap of WSe2 to take into account the band movement in graphene, the height of the Schottky barrier at the graphene-to-WSe2 contact was extracted to be 0.38 eV for the electron injection into the conduction band and 0.22 eV for the hole injection into the valence band at threshold bias condition. Figure 2e,f shows the partially top-gated transfer characteristics of the same TFT with h-BN as the gate dielectric and graphene as the gate electrode corresponding to two diﬀerent biasing condition of the back gate, VBG = 10 V and VBG
power and also make them more scalable. In this article, we experimentally demonstrate all 2D TFTs with monolayer graphene as metal electrodes, 3−4 atomic layers of h-BN as the gate dielectric and bilayers of WSe2 as the semiconducting channel material. We extracted electron mobility of 34 cm2/(V s) and hole mobility of 45 cm2/(V s) that exceed the conventional a-Si mobility (0.5−1 cm2/(V s)) by a factor of ∼100.24 The current ON−OFF ratio was found to be more than 107. We also report low contact resistance of 1.4 kΩ-μm. When fabricated on ﬂexible polyethylene terephthalate (PET) substrate, our active device stack of WSe2−hBN−graphene was found to be more than 88% transparent over the entire visible spectrum and the device characteristics were unaltered for inplane mechanical strain of up to 2%. The device also demonstrated temperature stability over 77−400 K. Fabrication of TFTs on silicon platforms as well as on ﬂexible polyethylene terephthalate (PET) substrates involved similar process ﬂows. WSe2 ﬂakes were micromechanically exfoliated using standard scotch tape technique while large area chemical vapor deposition grown monolayer graphene and few layer hBN were transferred on to the desired substrate. Optical lithography and reactive ion etching (RIE) were used for patterning purposes and electron beam evaporation was used for contact pads metallization (see the Supporting Information for the detailed fabrication process ﬂow). Figure 1a shows the false color SEM image of an all 2D TFT on 20 nm SiO2 substrate with highly doped Si as the back gate. Figure 1b,c, respectively, shows the three-dimensional cartoon and the cross sectional view of our device. Figure 2a shows the back-gated transfer characteristics of an all 2D TFT with bilayer WSe2 ﬂake as the channel material and graphene as the source/drain contact electrodes. Note that all the graphene electrodes are connected to metal pads at both ends to ensure uniform potential landscape across the entire graphene contacts (Figure 1b). An interesting feature of graphene contact is that, unlike conventional metal electrodes, the Fermi level of graphene responds to the back gate bias in spite of the charge screening by the WSe2 channel underneath the contacts. Figure 2b shows the transfer characteristics of a graphene ﬁeld eﬀect transistor (GFET) with underlying WSe2 as the screening layer. The characteristic is very similar to conventional GFET devices which clearly suggest that the 2862
dx.doi.org/10.1021/nl5009037 | Nano Lett. 2014, 14, 2861−2866
Figure 2. (a) Back gate transfer characteristics of a WSe2TFT with graphene as contact electrodes. Inset shows the cross section of the device. (b) Back gate transfer characteristics of a graphene FET with underlying WSe2 screening layer. Inset shows the false color SEM image and the cross section of the device. (c) Band movement (ΨGRAPHENE) in graphene in response to applied back gate bias. (d) Band alignment at graphene to WSe2 contact interface at diﬀerent back gate bias conditions shown in (a). (e,f) Top gate transfer characteristics of all 2D TFT corresponding to two diﬀerent back gate biases, VBG = 10 V and VBG = −10 V, respectively.
the trans-conductance, μ is the ﬁeld eﬀect mobility, and W and L are the channel width and the channel length, respectively, COX = εOX/dOX, where εOX is the dielectric constant and dOX is the thickness of the gate oxide, dOX = 3 nm and for h-BN, εOX = 6 × 10−11, which gives COX ∼ 3.10−2 F/m2, and ﬁnally L ∼ 5 μm) from the back-gated device characteristics. The ﬁeld-eﬀect mobility values were found to be 24 and 45 cm2/(V s) for electrons and holes, respectively. The reader should note that the mobility of amorphous Si is in the range of 0.5−1 cm2/(V
= −10 V respectively. For negative back gate biases, the WSe2 ﬂake is electrostatically p-doped and hence the top gated device exhibits p-FET characteristics, while for positive back gate biases the WSe2 ﬂake is electrostatically n-doped and hence the top gated device exhibits n-FET characteristics. The subthreshold slope was found to be ∼90 mV/decade for the p-FET and ∼130 mV/decade for the n-FET. The ﬁeld eﬀect mobility values were extracted using the conventional equation for gm = μCOX(W/L)VDS (where gm is 2863
dx.doi.org/10.1021/nl5009037 | Nano Lett. 2014, 14, 2861−2866
Figure 3. (a) Thinnest ﬁeld eﬀect transistor on ﬂexible PET substrate. (b) Transfer characteristics and (c) output characteristics of the TFT. (d) Experimental setup to measure the strain eﬀect. (e) Device characteristics under strain and (f) transparency of the TFT and its individual components.
LEDs, which will reduce cost, power dissipation, as well as open up avenues for innovative circuit design. The drive current is also important in the context of LCDs. The charging time of a pixel is inversely proportional to the drive (charging) current (τ = VDDCPIXEL/IDRIVE, where τ is the charging time, VDD is the supply voltage, and CPIXEL is the pixel capacitance). For a standard pixel capacitance in the range of 0.1−1pF, our all 2D TFTs will have a charging time of 0.1−1 μs. The resolution of an LCD (β = VDDCPARA/CPIXEL, where CPARA is the parasitic capacitance) can also be signiﬁcantly enhanced by using our all 2D TFT. For a standard parasitic capacitance of 50 fF, resolution of 5−50 mV can be achieved. Finally a ﬁgure of merit (γ = τ−1 β−1) as high as 108−1010 can be obtained which is 2−4 orders of magnitude higher than the state of the art a-Si TFTs. One of the major reasons for fabricating our all 2D TFT on silicon platform is to demonstrate high degree of compatibility with the conventional CMOS technology. As the fundamental limitations do not allow Si to scale below 10 nm technology node without compromising sevelry on the device performance, low-dimensional materials, especially 2D semiconducting transistion metal dichalcogenides (TMDs) will become more and more relevant in the context of high-performance CMOS as well. Our earlier studies related to channel length scaling, good quality contact formation, and layer thickness optimization of TMDs has shown a lot of promise.32−35 We have also implemented low power device concepts like tunneling FETs with the TMDs. There is a widespread concern about the low mobility values of the TMDs impacting the ON state performance of FETs.36 However, one should remember that for technology nodes beyond 10 nm the devices will be dominated by ballistic transport and hence the more important parameters are going to be the carrier injection velocity and
s) while the mobility of most of the organic semiconductors is